Feb 5, 2013 - Graphene, as a single layer of carbon atoms arranged packed densely in .... In order to examine the the size-dependent trends of properties for ...
Graphene nanoflakes - structural and electronic properties A. Kuc and T. Heine School of Engineering and Science, Jacobs University Bremen,
arXiv:1302.0964v1 [cond-mat.mtrl-sci] 5 Feb 2013
Campus Ring 1, 28759 Bremen, Germany G. Seifert Physikalische Chemie, Technische Universit¨ at, Bergstrasse 66b, 01062 Dresden, Germany
Abstract The structures, cohesive energies and HOMO-LUMO gaps of graphene nanoflakes and corresponding polycyclic aromatic hydrocarbons for a large variety of size and topology are investigated at the density functional based tight-binding level. Polyacene-like and honeycomb-like graphene nanoflakes were chosen as the topological limit structures. The influence of unsaturated edge atoms and dangling bonds on the stability is discussed. Our survey shows a linear trend for the cohesive energy as function of Ns /N (N − total number of atoms and Ns is number of edge atoms). For the HOMO-LUMO gap the trends are more complex and include also the topology of the edges. Keywords: Graphene Nanoflakes, Polycyclic Aromatic Hydrocarbons, Topology Trends, Energetic Stability, Electronic Properties, DFTB
Graphene, as a single layer of carbon atoms arranged packed densely in a two-dimensional honeycomb crystal lattice, has attracted an enormous interest in the area of solid state electronics and composite materials, due to its high mechanical, thermal and chemical stability and excellent electronic properties. Graphene nanoribbons (GNRs) and nanoflakes (GNFs), that are finite in both dimensions, can be considered as fragments or molecular subunits of graphene. Since their initial successful fabrication,1 the dimensions of GNRs and GNFs have rapidly reduced from the microscale down to nanometer sizes either by top-down2 or bottom-up3,4 approaches. This gave a possibility to explore low-dimensional transport and perspective for carbon-based nanoelectronics. Depending on the size and shape, GNFs possess the ability to form ordered columnar mesophases.5 Since the basic functional components of future electronics and spiroelectronics devices are required to be on the nanometer scale it is important to understand the properties of GNFs and their saturated counterparts, polycyclic aromatic hydrocarbons (PAHs). Isolated GNFs and GNRs can be presently produced using different experimental approaches. The bottom-up approach by thermal annealing nanographene molecules results in a conductive graphene film.4 Alternatively, nanographene can be produced by soft-landing of ions generated by solvent-free matrix assisted laser desorption/ionisation.6 The product is transfered to the gas phase, purified and adsorbed at surfaces. As top-down-techniques, GNRs with widths varying from several tens of nanometers down to 2 nm have been fabricated either by etching7–9 or by means of chemical treatment of graphene or graphite.2 It has been reported that GNRs with certain edge chirality would open the band gap.10 GNFs with controlled thicknesses have been isolated in solution using density gradient ultracentrifugation.11 Cong et al12 . have fabricated arrays of graphene nanodiscs (GNDs) using nanosphere lithography (GNDs are GNFs with smooth edges and spherical shape). Fabrication of GNRs with smooth edges is essential for many applications, however, it is difficult to produce such edges by conventional physico-chemical methods. Jia et al.13 have shown that an efficient edge-reconstruction process, at the atomic scale, can be obtained for graphitic nanoribbons by Joule heating using an integrated transmission electron microscope-scanning tunnelling microscope (TEM-STM) system. 2
Very recently, few groups have independently reported very elegant methods for GNR production.14–16 The methods are based on the longitudinal unzipping of multi-walled CNTs and involve an Ar plasma etching of the nanotubes. These procedures are simple and inexpensive, and lead to GNRs with well-defined widths and edge structures. It is widely known that stable GNFs with sizes C3 –C10 form linear conformations, C11 – C20 form annular structures and Cn s with n > 20 form fullerenes.17–19 However, it appears that so far little is known on the stability, structure and properties of larger (planar) carbon nanostructures, and a computational study is timely. Graphite and graphene are zero-gap semiconductors. If carbon particles are reduced in size to a level where quantum effects are significant, large energy gaps may appear.20 Indeed, as large as 8.5 eV energy gaps have been predicted for clusters with few carbon atoms,21 while gaps below 2 eV were found for carbon cages composed of up to 80 carbon atoms.22–24 The knowledge and understanding of the size-tuned properties, e.g. binding energy and HOMO-LUMO gap, would make carbon particles interesting candidates for applications in nanotechnology.
FIG. 1: Exemplary graphene nanoflakes isomers considered for C26 .
In this paper, we focus on small and medium neutral GNFs and corresponding PAHs. We have restricted our calculations to even number of atoms, as well as to planar sixfold 3
ring systems (polyhexe structures; see Fig. 1). The determination of topologically distinct structures (isomers) is difficult, as the number of isomers is strictly related to the number of atoms (n) and increases rapidly with increasing n. As an example, for the molecular formula C6 H6 , about 330 isomers can be written, considering the geometrical- and stereo-isomers.25 The complete set of isomers for any graphene flage can be created using graph theory.26,27 In this work, we do not aim to investigate all possible graphene flake structures, instead we want to derive trends in stability and electronic structure on the basis of an extensive survey of flake structures inhibiting different molecular weight and topology. We have created a number of possible isomers for structures with N=6–34, 38, 42, 50, 54, 60, and 74 (N is the number of carbon atoms). For some specific topologies, e.g. triangles, nanoribbons (stripes) or circular flakes, the number of atoms was up to 220. Since the number of isomers rapidly increases with increasing N the completeness in selection was related only to the smallest structures (N